# Electronic Supplementary Material (ESI) for ChemComm.
# This journal is © The Royal Society of Chemistry 2023

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_1
_database_code_depnum_ccdc_archive 'CCDC 2231626'
loop_
_audit_author_name
_audit_author_address
'Miriding Mutailipu'
;Chinese academic of science
China
;
_audit_update_record             
;
2022-12-20 deposited with the CCDC.	2023-01-23 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-97
_chemical_name_systematic        
; 
 ? 
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'H2 B3 Cs F2 O5'
_chemical_formula_weight         285.36

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
B B 0.0013 0.0007 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           Monoclinic
_symmetry_space_group_name_H-M   P2(1)/c

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'

_cell_length_a                   7.4498(5)
_cell_length_b                   5.9711(4)
_cell_length_c                   15.5448(12)
_cell_angle_alpha                90.00
_cell_angle_beta                 100.466(3)
_cell_angle_gamma                90.00
_cell_volume                     679.98(8)
_cell_formula_units_Z            4
_cell_measurement_temperature    300(2)
_cell_measurement_reflns_used    2831
_cell_measurement_theta_min      2.78
_cell_measurement_theta_max      25.70

_exptl_crystal_description       block
_exptl_crystal_colour            colourless
_exptl_crystal_size_max          0.13
_exptl_crystal_size_mid          0.12
_exptl_crystal_size_min          0.10
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    2.787
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             520
_exptl_absorpt_coefficient_mu    5.451
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_correction_T_min  0.5376
_exptl_absorpt_correction_T_max  0.6117
_exptl_absorpt_process_details   face-indexed

_exptl_special_details           
; 
 ? 
;

_diffrn_ambient_temperature      300(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_detector_area_resol_mean ?
_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            11704
_diffrn_reflns_av_R_equivalents  0.0758
_diffrn_reflns_av_sigmaI/netI    0.0374
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_k_min       -7
_diffrn_reflns_limit_k_max       7
_diffrn_reflns_limit_l_min       -20
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_theta_min         2.66
_diffrn_reflns_theta_max         27.51
_reflns_number_total             1568
_reflns_number_gt                1248
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       'Bruker SMART'
_computing_cell_refinement       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    'SHELXL-97 (Sheldrick, 1997)'
_computing_publication_material  'SHELXL-97 (Sheldrick, 1997)'

_refine_special_details          
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0127P)²+0.5597P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    mixed
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       ?
_refine_ls_number_reflns         1568
_refine_ls_number_parameters     108
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0475
_refine_ls_R_factor_gt           0.0299
_refine_ls_wR_factor_ref         0.0501
_refine_ls_wR_factor_gt          0.0463
_refine_ls_goodness_of_fit_ref   1.067
_refine_ls_restrained_S_all      1.067
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Cs1 Cs 0.09132(3) 0.27907(4) 0.114890(19) 0.03744(10) Uani 1 1 d . . .
B1 B 0.2194(6) 0.2714(8) 0.3674(3) 0.0321(11) Uani 1 1 d . . .
B2 B 0.4225(6) 0.5727(8) 0.3396(3) 0.0334(11) Uani 1 1 d . . .
B3 B 0.5452(6) 0.2749(8) 0.4332(3) 0.0324(11) Uani 1 1 d . . .
F1 F 0.1713(3) 0.1065(4) 0.30042(17) 0.0441(6) Uani 1 1 d . . .
F2 F 0.0708(3) 0.2894(4) 0.41032(17) 0.0441(6) Uani 1 1 d . . .
O1 O 0.2539(3) 0.4820(4) 0.32794(19) 0.0350(7) Uani 1 1 d . . .
O2 O 0.5726(3) 0.4655(4) 0.3882(2) 0.0370(7) Uani 1 1 d . . .
O3 O 0.3762(3) 0.1878(4) 0.42836(19) 0.0341(7) Uani 1 1 d . . .
O4 O 0.6933(4) 0.1821(6) 0.4847(2) 0.0443(8) Uani 1 1 d . . .
O5 O 0.4613(4) 0.7719(5) 0.3063(2) 0.0463(9) Uani 1 1 d . . .
H1 H 0.377(6) 0.837(7) 0.287(3) 0.034(14) Uiso 1 1 d . . .
H2 H 0.677(7) 0.076(9) 0.511(4) 0.07(2) Uiso 1 1 d . . .


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Cs1 F1 3.018(3) . ?
Cs1 O2 3.134(3) 2_645 ?
Cs1 F2 3.161(2) 2_545 ?
Cs1 F2 3.182(3) 4_565 ?
Cs1 F1 3.212(3) 2 ?
Cs1 F2 3.275(2) 2 ?
Cs1 O4 3.280(3) 4_465 ?
Cs1 O5 3.336(3) 2_645 ?
Cs1 O1 3.374(3) 2_545 ?
Cs1 O4 3.415(4) 2_655 ?
Cs1 O1 3.528(3) . ?
Cs1 B2 3.769(5) 2_645 ?
B1 F2 1.397(5) . ?
B1 F1 1.430(5) . ?
B1 O1 1.442(5) . ?
B1 O3 1.453(5) . ?
B1 Cs1 3.783(4) 2_545 ?
B1 Cs1 3.854(5) 2 ?
B2 O5 1.349(5) . ?
B2 O1 1.350(5) . ?
B2 O2 1.387(5) . ?
B2 Cs1 3.769(5) 2_655 ?
B3 O3 1.352(5) . ?
B3 O4 1.358(5) . ?
B3 O2 1.370(5) . ?
F1 Cs1 3.212(3) 2_545 ?
F2 Cs1 3.161(2) 2 ?
F2 Cs1 3.182(3) 4_566 ?
F2 Cs1 3.275(2) 2_545 ?
O1 Cs1 3.374(3) 2 ?
O2 Cs1 3.134(3) 2_655 ?
O4 Cs1 3.280(3) 4_666 ?
O4 Cs1 3.415(4) 2_645 ?
O4 H2 0.78(5) . ?
O5 Cs1 3.336(3) 2_655 ?
O5 H1 0.75(4) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
F1 Cs1 O2 77.95(8) . 2_645 ?
F1 Cs1 F2 78.89(6) . 2_545 ?
O2 Cs1 F2 74.56(6) 2_645 2_545 ?
F1 Cs1 F2 151.21(7) . 4_565 ?
O2 Cs1 F2 78.54(7) 2_645 4_565 ?
F2 Cs1 F2 79.01(7) 2_545 4_565 ?
F1 Cs1 F1 81.10(5) . 2 ?
O2 Cs1 F1 156.60(7) 2_645 2 ?
F2 Cs1 F1 111.50(6) 2_545 2 ?
F2 Cs1 F1 124.43(6) 4_565 2 ?
F1 Cs1 F2 115.88(7) . 2 ?
O2 Cs1 F2 146.34(7) 2_645 2 ?
F2 Cs1 F2 136.19(7) 2_545 2 ?
F2 Cs1 F2 92.88(6) 4_565 2 ?
F1 Cs1 F2 40.88(6) 2 2 ?
F1 Cs1 O4 127.80(8) . 4_465 ?
O2 Cs1 O4 131.91(8) 2_645 4_465 ?
F2 Cs1 O4 72.95(7) 2_545 4_465 ?
F2 Cs1 O4 61.23(8) 4_565 4_465 ?
F1 Cs1 O4 70.14(8) 2 4_465 ?
F2 Cs1 O4 65.67(7) 2 4_465 ?
F1 Cs1 O5 68.55(8) . 2_645 ?
O2 Cs1 O5 41.42(7) 2_645 2_645 ?
F2 Cs1 O5 111.56(7) 2_545 2_645 ?
F2 Cs1 O5 103.21(7) 4_565 2_645 ?
F1 Cs1 O5 119.98(7) 2 2_645 ?
F2 Cs1 O5 112.21(7) 2 2_645 ?
O4 Cs1 O5 163.38(9) 4_465 2_645 ?
F1 Cs1 O1 66.19(7) . 2_545 ?
O2 Cs1 O1 109.85(7) 2_645 2_545 ?
F2 Cs1 O1 41.74(6) 2_545 2_545 ?
F2 Cs1 O1 107.17(6) 4_565 2_545 ?
F1 Cs1 O1 70.23(6) 2 2_545 ?
F2 Cs1 O1 103.79(6) 2 2_545 ?
O4 Cs1 O1 63.43(8) 4_465 2_545 ?
O5 Cs1 O1 130.95(8) 2_645 2_545 ?
F1 Cs1 O4 130.26(7) . 2_655 ?
O2 Cs1 O4 88.36(8) 2_645 2_655 ?
F2 Cs1 O4 142.75(8) 2_545 2_655 ?
F2 Cs1 O4 65.08(7) 4_565 2_655 ?
F1 Cs1 O4 97.36(7) 2 2_655 ?
F2 Cs1 O4 58.91(7) 2 2_655 ?
O4 Cs1 O4 96.72(7) 4_465 2_655 ?
O5 Cs1 O4 69.82(8) 2_645 2_655 ?
O1 Cs1 O4 158.95(7) 2_545 2_655 ?
F1 Cs1 O1 41.04(6) . . ?
O2 Cs1 O1 94.63(7) 2_645 . ?
F2 Cs1 O1 119.50(6) 2_545 . ?
F2 Cs1 O1 158.15(6) 4_565 . ?
F1 Cs1 O1 62.42(6) 2 . ?
F2 Cs1 O1 81.31(6) 2 . ?
O4 Cs1 O1 132.26(8) 4_465 . ?
O5 Cs1 O1 60.66(7) 2_645 . ?
O1 Cs1 O1 94.67(5) 2_545 . ?
O4 Cs1 O1 94.25(7) 2_655 . ?
F1 Cs1 B2 72.11(10) . 2_645 ?
O2 Cs1 B2 20.67(8) 2_645 2_645 ?
F2 Cs1 B2 93.06(8) 2_545 2_645 ?
F2 Cs1 B2 90.91(9) 4_565 2_645 ?
F1 Cs1 B2 139.29(9) 2 2_645 ?
F2 Cs1 B2 130.36(8) 2 2_645 ?
O4 Cs1 B2 150.35(10) 4_465 2_645 ?
O5 Cs1 B2 20.75(8) 2_645 2_645 ?
O1 Cs1 B2 122.09(9) 2_545 2_645 ?
O4 Cs1 B2 78.52(9) 2_655 2_645 ?
O1 Cs1 B2 77.39(9) . 2_645 ?
F2 B1 F1 106.6(3) . . ?
F2 B1 O1 110.8(3) . . ?
F1 B1 O1 109.4(4) . . ?
F2 B1 O3 109.1(3) . . ?
F1 B1 O3 107.7(3) . . ?
O1 B1 O3 113.1(3) . . ?
F2 B1 Cs1 58.41(19) . 2_545 ?
F1 B1 Cs1 56.09(19) . 2_545 ?
O1 B1 Cs1 150.2(3) . 2_545 ?
O3 B1 Cs1 96.6(2) . 2_545 ?
F2 B1 Cs1 50.74(18) . 2 ?
F1 B1 Cs1 121.3(2) . 2 ?
O1 B1 Cs1 60.0(2) . 2 ?
O3 B1 Cs1 130.2(3) . 2 ?
Cs1 B1 Cs1 102.86(11) 2_545 2 ?
O5 B2 O1 124.1(4) . . ?
O5 B2 O2 114.1(4) . . ?
O1 B2 O2 121.8(4) . . ?
O5 B2 Cs1 61.2(2) . 2_655 ?
O1 B2 Cs1 174.6(3) . 2_655 ?
O2 B2 Cs1 52.90(19) . 2_655 ?
O3 B3 O4 121.6(4) . . ?
O3 B3 O2 121.0(4) . . ?
O4 B3 O2 117.4(4) . . ?
B1 F1 Cs1 116.1(2) . . ?
B1 F1 Cs1 102.2(2) . 2_545 ?
Cs1 F1 Cs1 124.77(8) . 2_545 ?
B1 F2 Cs1 109.3(2) . 2 ?
B1 F2 Cs1 124.7(2) . 4_566 ?
Cs1 F2 Cs1 100.99(7) 2 4_566 ?
B1 F2 Cs1 100.3(2) . 2_545 ?
Cs1 F2 Cs1 136.19(7) 2 2_545 ?
Cs1 F2 Cs1 87.12(6) 4_566 2_545 ?
B2 O1 B1 121.8(3) . . ?
B2 O1 Cs1 119.3(3) . 2 ?
B1 O1 Cs1 98.2(2) . 2 ?
B2 O1 Cs1 114.6(3) . . ?
B1 O1 Cs1 92.4(2) . . ?
Cs1 O1 Cs1 106.24(7) 2 . ?
B3 O2 B2 118.8(3) . . ?
B3 O2 Cs1 134.2(2) . 2_655 ?
B2 O2 Cs1 106.4(2) . 2_655 ?
B3 O3 B1 122.3(3) . . ?
B3 O4 Cs1 151.8(3) . 4_666 ?
B3 O4 Cs1 114.7(3) . 2_645 ?
Cs1 O4 Cs1 83.28(7) 4_666 2_645 ?
B3 O4 H2 117(4) . . ?
Cs1 O4 H2 87(4) 4_666 . ?
Cs1 O4 H2 78(4) 2_645 . ?
B2 O5 Cs1 98.0(3) . 2_655 ?
B2 O5 H1 113(3) . . ?
Cs1 O5 H1 147(3) 2_655 . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
F2 B1 F1 Cs1 108.2(3) . . . . ?
O1 B1 F1 Cs1 -11.5(4) . . . . ?
O3 B1 F1 Cs1 -134.8(2) . . . . ?
Cs1 B1 F1 Cs1 139.1(2) 2_545 . . . ?
Cs1 B1 F1 Cs1 54.5(3) 2 . . . ?
F2 B1 F1 Cs1 -30.9(3) . . . 2_545 ?
O1 B1 F1 Cs1 -150.6(2) . . . 2_545 ?
O3 B1 F1 Cs1 86.1(3) . . . 2_545 ?
Cs1 B1 F1 Cs1 -84.6(2) 2 . . 2_545 ?
O2 Cs1 F1 B1 118.5(3) 2_645 . . . ?
F2 Cs1 F1 B1 -165.1(3) 2_545 . . . ?
F2 Cs1 F1 B1 154.4(2) 4_565 . . . ?
F1 Cs1 F1 B1 -51.0(2) 2 . . . ?
F2 Cs1 F1 B1 -28.9(3) 2 . . . ?
O4 Cs1 F1 B1 -107.2(3) 4_465 . . . ?
O5 Cs1 F1 B1 76.2(2) 2_645 . . . ?
O1 Cs1 F1 B1 -123.2(3) 2_545 . . . ?
O4 Cs1 F1 B1 41.2(3) 2_655 . . . ?
O1 Cs1 F1 B1 6.7(2) . . . . ?
B2 Cs1 F1 B1 98.0(3) 2_645 . . . ?
O2 Cs1 F1 Cs1 -112.66(10) 2_645 . . 2_545 ?
F2 Cs1 F1 Cs1 -36.28(9) 2_545 . . 2_545 ?
F2 Cs1 F1 Cs1 -76.77(16) 4_565 . . 2_545 ?
F1 Cs1 F1 Cs1 77.85(13) 2 . . 2_545 ?
F2 Cs1 F1 Cs1 99.94(10) 2 . . 2_545 ?
O4 Cs1 F1 Cs1 21.67(14) 4_465 . . 2_545 ?
O5 Cs1 F1 Cs1 -154.94(12) 2_645 . . 2_545 ?
O1 Cs1 F1 Cs1 5.61(8) 2_545 . . 2_545 ?
O4 Cs1 F1 Cs1 169.99(9) 2_655 . . 2_545 ?
O1 Cs1 F1 Cs1 135.58(15) . . . 2_545 ?
B2 Cs1 F1 Cs1 -133.20(12) 2_645 . . 2_545 ?
F1 B1 F2 Cs1 -117.2(3) . . . 2 ?
O1 B1 F2 Cs1 1.7(4) . . . 2 ?
O3 B1 F2 Cs1 126.8(3) . . . 2 ?
Cs1 B1 F2 Cs1 -147.16(17) 2_545 . . 2 ?
F1 B1 F2 Cs1 123.6(3) . . . 4_566 ?
O1 B1 F2 Cs1 -117.5(3) . . . 4_566 ?
O3 B1 F2 Cs1 7.6(4) . . . 4_566 ?
Cs1 B1 F2 Cs1 93.65(19) 2_545 . . 4_566 ?
Cs1 B1 F2 Cs1 -119.2(3) 2 . . 4_566 ?
F1 B1 F2 Cs1 30.0(3) . . . 2_545 ?
O1 B1 F2 Cs1 148.9(3) . . . 2_545 ?
O3 B1 F2 Cs1 -86.0(3) . . . 2_545 ?
Cs1 B1 F2 Cs1 147.16(17) 2 . . 2_545 ?
O5 B2 O1 B1 -178.0(4) . . . . ?
O2 B2 O1 B1 1.7(7) . . . . ?
Cs1 B2 O1 B1 0(4) 2_655 . . . ?
O5 B2 O1 Cs1 -55.3(6) . . . 2 ?
O2 B2 O1 Cs1 124.4(4) . . . 2 ?
Cs1 B2 O1 Cs1 123(3) 2_655 . . 2 ?
O5 B2 O1 Cs1 72.3(5) . . . . ?
O2 B2 O1 Cs1 -108.1(4) . . . . ?
Cs1 B2 O1 Cs1 -110(4) 2_655 . . . ?
F2 B1 O1 B2 130.6(4) . . . . ?
F1 B1 O1 B2 -112.2(4) . . . . ?
O3 B1 O1 B2 7.8(6) . . . . ?
Cs1 B1 O1 B2 -167.1(5) 2_545 . . . ?
Cs1 B1 O1 B2 132.2(4) 2 . . . ?
F2 B1 O1 Cs1 -1.5(3) . . . 2 ?
F1 B1 O1 Cs1 115.6(3) . . . 2 ?
O3 B1 O1 Cs1 -124.4(3) . . . 2 ?
Cs1 B1 O1 Cs1 60.8(6) 2_545 . . 2 ?
F2 B1 O1 Cs1 -108.3(3) . . . . ?
F1 B1 O1 Cs1 8.8(3) . . . . ?
O3 B1 O1 Cs1 128.9(3) . . . . ?
Cs1 B1 O1 Cs1 -46.0(6) 2_545 . . . ?
Cs1 B1 O1 Cs1 -106.79(9) 2 . . . ?
F1 Cs1 O1 B2 120.8(3) . . . . ?
O2 Cs1 O1 B2 55.1(3) 2_645 . . . ?
F2 Cs1 O1 B2 130.0(3) 2_545 . . . ?
F2 Cs1 O1 B2 -15.4(3) 4_565 . . . ?
F1 Cs1 O1 B2 -129.7(3) 2 . . . ?
F2 Cs1 O1 B2 -91.3(3) 2 . . . ?
O4 Cs1 O1 B2 -136.7(3) 4_465 . . . ?
O5 Cs1 O1 B2 30.4(3) 2_645 . . . ?
O1 Cs1 O1 B2 165.5(2) 2_545 . . . ?
O4 Cs1 O1 B2 -33.6(3) 2_655 . . . ?
B2 Cs1 O1 B2 43.6(2) 2_645 . . . ?
F1 Cs1 O1 B1 -6.0(2) . . . . ?
O2 Cs1 O1 B1 -71.7(2) 2_645 . . . ?
F2 Cs1 O1 B1 3.2(2) 2_545 . . . ?
F2 Cs1 O1 B1 -142.2(2) 4_565 . . . ?
F1 Cs1 O1 B1 103.5(2) 2 . . . ?
F2 Cs1 O1 B1 142.0(2) 2 . . . ?
O4 Cs1 O1 B1 96.6(2) 4_465 . . . ?
O5 Cs1 O1 B1 -96.4(2) 2_645 . . . ?
O1 Cs1 O1 B1 38.7(2) 2_545 . . . ?
O4 Cs1 O1 B1 -160.4(2) 2_655 . . . ?
B2 Cs1 O1 B1 -83.2(2) 2_645 . . . ?
F1 Cs1 O1 Cs1 -105.29(11) . . . 2 ?
O2 Cs1 O1 Cs1 -170.97(8) 2_645 . . 2 ?
F2 Cs1 O1 Cs1 -96.10(8) 2_545 . . 2 ?
F2 Cs1 O1 Cs1 118.53(15) 4_565 . . 2 ?
F1 Cs1 O1 Cs1 4.23(6) 2 . . 2 ?
F2 Cs1 O1 Cs1 42.68(7) 2 . . 2 ?
O4 Cs1 O1 Cs1 -2.73(13) 4_465 . . 2 ?
O5 Cs1 O1 Cs1 164.32(10) 2_645 . . 2 ?
O1 Cs1 O1 Cs1 -60.58(10) 2_545 . . 2 ?
O4 Cs1 O1 Cs1 100.33(8) 2_655 . . 2 ?
B2 Cs1 O1 Cs1 177.56(10) 2_645 . . 2 ?
O3 B3 O2 B2 2.0(6) . . . . ?
O4 B3 O2 B2 -175.8(4) . . . . ?
O3 B3 O2 Cs1 172.3(3) . . . 2_655 ?
O4 B3 O2 Cs1 -5.6(6) . . . 2_655 ?
O5 B2 O2 B3 172.6(4) . . . . ?
O1 B2 O2 B3 -7.1(7) . . . . ?
Cs1 B2 O2 B3 172.7(4) 2_655 . . . ?
O5 B2 O2 Cs1 -0.1(5) . . . 2_655 ?
O1 B2 O2 Cs1 -179.8(4) . . . 2_655 ?
O4 B3 O3 B1 -173.9(4) . . . . ?
O2 B3 O3 B1 8.4(6) . . . . ?
F2 B1 O3 B3 -136.6(4) . . . . ?
F1 B1 O3 B3 108.1(4) . . . . ?
O1 B1 O3 B3 -12.9(6) . . . . ?
Cs1 B1 O3 B3 164.6(3) 2_545 . . . ?
Cs1 B1 O3 B3 -82.3(5) 2 . . . ?
O3 B3 O4 Cs1 -144.5(4) . . . 4_666 ?
O2 B3 O4 Cs1 33.3(9) . . . 4_666 ?
O3 B3 O4 Cs1 89.6(5) . . . 2_645 ?
O2 B3 O4 Cs1 -92.6(4) . . . 2_645 ?
O1 B2 O5 Cs1 179.8(4) . . . 2_655 ?
O2 B2 O5 Cs1 0.1(4) . . . 2_655 ?

_diffrn_measured_fraction_theta_max 0.999
_diffrn_reflns_theta_full        27.51
_diffrn_measured_fraction_theta_full 0.999
_refine_diff_density_max         0.570
_refine_diff_density_min         -0.588
_refine_diff_density_rms         0.125
